Lecture Outline Crystallography


 Polly McDaniel
 3 years ago
 Views:
Transcription
1 Lecture Outline Crystallography Short and long range Order Poly and single crystals, anisotropy, polymorphy Allotropic and Polymorphic Transitions Lattice, Unit Cells, Basis, Packing, Density, and Crystal Structures Points, Directions, and Planes in the Unit Cell Structures with more than one atoms per lattice point Interstitial Sites Ionic Crystal Structures Covalent Crystal Structures Metallic Crystal structures Diffraction and modern microscopy 1
2 Lowest ENERGY state at each temperature Non dense, random packing There is still short range order typical neighbor bond energy Energy typical neighbor bond length r Dense, regular packing Energy There is long range order in addition to short range order typical neighbor bond energy typical neighbor bond length r Dense, regularpacked structures tend to have lower energy, of course everything depends on temperature, at low enough temperatures many materials crystallize
3 MATERIALS AND PACKING Crystalline materials... atoms pack in periodic, 3D arrays typical of: metals many ceramics  semiconductors some polymers Glass is actually a cold melt, over long enough times, it crystallizes, old church windows are thicker at the bottom Noncrystalline materials... atoms have no periodic packing occurs for: complex structures  rapid cooling Si One of many forms of crystalline SiO Oxygen "Amorphous" = Noncrystalline noncrystalline SiO Quartz glass, a cold melt 3
4 Classification of materials based on type of atomic order. 4
5 Levels of atomic arrangements in materials: (a)inert monoatomic gases have no regular ordering of atoms: (b,c) Some materials, including water vapor, nitrogen gas, amorphous silicon and silicate glass have shortrange order. (d) Metals, alloys, many ceramics, semiconductors and some polymers have regular ordering of atoms/ions that extends through the material = crystals 5
6 Basic Si0 tetrahedron in silicate glass. Xray diffraction shows only short range order. Note that this cannot exist in quartz at room temperature, there the tetrahedron is distorted resulting in pronounced anisotropy effects such as piezoelectricity. In ßcristobalite, a high temperature phase of quartz, we have an undistorted tetrahedron again, Xray diffraction shows long range order 6
7 Again there are different crystallograp hic phases, i.e. long range order structures until the crystal melts and only short range order remains 7
8 Atomic arrangements in (a) Amorphous silicon with H (b) Crystalline silicon. Note the variation in the interatomic distance for amorphous silicon, but there still is shortrange order 8
9 POLYCRYSTALS Most engineering materials are polycrystalline! 1 mm NbHfW plate with an electron beam weld. Each "grain" is a single crystal. If crystals are randomly oriented, component properties are not directional, but frequently we have texture, preferred orientation of polycrystals resulting in pronounced anisotropy Crystal sizes range from 1 nm to cm, (i.e., from a few to millions of atomic layers). 9
10 SINGLE versus POLYCRYSTALS Single (Mono)crystals  Properties vary with direction: anisotropy.  Example: the modulus of elasticity (E) in BCC iron: E (diagonal) = 73 GPa Polycrystals  Properties may/may not vary with direction, depending on degree of texture.  If grains are randomly oriented: isotropic. (E poly iron = 10 GPa)  If grains are textured, anisotropic. E (edge) = 15 GPa 00 µm 10
11 Allotropic and Polymorphic Transitions Allotropy  The characteristic of an element being able to exist in more than one crystal structure, depending on temperature and pressure. Polymorphism  Compounds exhibiting more than one type of crystal structure. Everything depends on temperature and pressure, e.g. coefficient of thermal expansion can, therefore, only be defined over a certain region of temperature 11
12 Covalently bonded layer Cubic crystal Covalently bonded network of atoms Layers bonded by van der Waals bonding Covalently bonded layer Hexagonal unit cell (a) Diamond unit cell (b) Graphite The FCC unit cell of the Buckminsterfullerene crystal. Each lattice point has a C 60 molecule Buckminsterfullerene (C 60 ) molecule (the "buckyball" molecule) (c) Buckminsterfullerene 1
13 13
14 U(X) = PE = mgh Metastable Unstable (Activated State) E A U U A* U A U B A A* B Stable X X A X A* X B System Coordinate, X = Position of Center of Mass Fig. 1.7: Tilting a filing cabinet from state A to its edge in state A* requires an energy E A. After reaching A*, the cabinet spontaneously drops to the stable position B. PE of state B is lower than A and therefore state B is more stable than A. 14
15 Example: heating and cooling of a hanging iron wire Demonstrates "polymorphism" Temperature, C The same group of atoms has more than one crystal structure. The actual structure depends on temperature and pressure Liquid BCC Stable longer 914 Tc 768 FCC Stable BCC Stable heat up cool down shorter! longer! magnet falls off shorter 15
16 Lattice, Unit Cells, Basis, and Crystal Structures Lattice  a 3D collection of points that divide space into smaller equally sized units. Basis  a group of atoms associated with a lattice point. This may be one single atom or a group of atoms. Unit cell  a subdivision of the lattice that still retains the overall characteristics of the entire lattice, contains at least one atom may contain many atoms. Atomic radius  apparent radius of an atom, typically calculated from the dimensions of the unit cell, using closepacked directions (depends upon type of bonding, coordination number, quantum mechanics). Packing factor  The fraction of space in a unit cell occupied by atoms. 16
17 The fourteen types of Bravais) lattices grouped in seven crystal systems: triclinic monocline rhombohedral = (trigonal) orthorhombic tetragonal hexagonal cubic 17
18 Definition of lattice parameters in cubic, orthorhombic, and hexagonal crystal systems. For cubic crystals, however, calculations are just like with Cartesian coordinates Note that angles are not always 90 degrees and coordination axis lengths are not necessarily all equal, as you know them to be from Cartesian coordinates 18
19 19
20 Lattice Points and Directions in the Unit Cell Millerindices  A shorthand notation to describe certain crystallographic directions and planes in a material. Lattice directions are in direct space and are denoted by [ ] brackets. A negative number is represented by a bar over the number. Directions of a form (also called family)  Crystallographic directions that all have the same characteristics, although their sense may be different. Denoted by <> brackets, they are symmetrically equivalent 0
21 Lattice Planes in the Unit Cell are an altogether different matter! Millerindices  A shorthand notation to describe certain crystallographic directions and planes in a material. Lattice planes are represented by the vector that is normal (perpendicular to them), these are 3D vectors in reciprocal (or dual) space (reciprocal space is nothing fancy  it is just a mathematical convenience!) Directions of a form (also called family) lattice planes that all have the same characteristics, although their sense may be different. Denoted by {} brackets, they are symmetrically equivalent. Now if the lattice point represents more than one point the front side and the back side of one and the same plane may have very different chemical properties as different atoms will be exposed, e.g. ZnS structure 1
22 We start with the coordinates of lattice points in order to define the Miller indices of lattice directions Coordinates of selected points in the unit cell. The number refers to the distance from the origin in terms of lattice parameters.
23 Determining Miller Indices of Directions Determine coordinates of two points that lie in direction of interest, u 1 v 1 w 1 and u v w calculations are simplified if the second point corresponds with the origin of the coordinate system Subtract coordinates of second point from those of first point u = u 1 u, v = v 1 v, w = w 1 w Clear fractions from the differences to give indices in lowest integer values. Write indices in [] brackets. Negative integer values are indicated with a bar over the integer, [uvw] and [uvw] are running in opposite directions 3
24 Direction A 1. Two points are 1, 0, 0, and 0, 0, 0. 1, 0, 0,  (0, 0, 0) = 1, 0, 0 3. No fractions to clear or integers to reduce 4. [100] Direction B 1. Two points are 1, 1, 1 and 0, 0, 0. 1, 1, 1,  (0, 0, 0) = 1, 1, 1 3. No fractions to clear or integers to reduce 4. [111] Direction C 1. Two points are 0, 0, 1 and 1/, 1, 0. 0, 0, 1 (1/, 1, 0) = 1/, 1, 1 3. (1/, 1, 1) = 1,, 4. [ 1 ] 4
25 Equivalency of crystallographic directions of a form in cubic systems. 5
26 6
27 Determining Miller Indices of Planes Identify the coordinate intersects of the plane, if plane is parallel to one of the axes, this intercept is taken to be infinite Take the reciprocal of the intercept Clear fractions, but do not reduce to lowest integers Cite in (h k l) parentheses Negative integer values are indicated with a bar over the integer (h k l) is the same plane as (h k l), just its back side 7
28 Plane A 1. x = 1, y = 1, z = 1.1/x = 1, 1/y = 1,1 /z = 1 3. No fractions to clear 4. (111) Plane B 1. The plane never intercepts the z axis, so x = 1, y =, and z =.1/x = 1, 1/y =1/, 1/z = 0 3. Clear fractions: 1/x =, 1/y = 1, 1/z = 0 4. (10) Plane C 1. We shall move the origin, since the plane passes through 0, 0, 0. Let s move the origin one lattice parameter in the ydirection. Then, x =, y = 1, and z =.1/x = 0, 1/y = 1, 1/z = 0 3. No fractions to clear. 4.(010) that seemed a bit arbitrary, we could have moved the origin in the y direction as well, then we would have gotten (010), which is just the back side of (010) 8
29 x intercept at a / z intercept at x z Unit cell b a c y Miller Indices (hkl ) : y intercept at b (a) Identification of a plane in a crystal z (010) (010) z (010) 1 (10) (010) x (010) y x (001) (110) y (100) z z (110) (111) (111) y y x y x (b) Various planes in the cubic lattice z 9
30 30
31 Drawing Direction and Plane [11] [10] Draw (a) the direction and (b) the plane in a cubic unit cell. Construction of a (a) direction and (b) plane within a unit cell 31
32 SOLUTION a. Because we know that we will need to move in the negative ydirection, let s locate the origin at 0, +1, 0. The tail of the direction will be located at this new origin. A second point on the direction can be determined by moving +1 in the xdirection, in the negative ydirection, and +1 in the z direction. [10] b. To draw in the plane, first take reciprocals of the indices to obtain the intercepts, that is: x = 1/ = 1/ y = 1/1 = 1 z = 1/0 = Since the xintercept is in a negative direction, and we wish to draw the plane within the unit cell, let s move the origin +1 in the xdirection to 1, 0, 0. Then we can locate the xintercept at 1/ and the yintercept at +1. The plane will be parallel to the zaxis. 3
33 Determining MillerBravais Indices for Planes and Directions in hexagonal system MillerBravais indices are obtained for crystallographic planes, directions, and points in hexagonal unit cells by using a fouraxis coordinate system. For planes (hkil), the index i = (h+k), i.e. h+k = i For directions [uvtw], we have also t = (u+v), i.e. u+v = t 33
34 MillerBravais indices for planes are straightforward, just as we obtained the intersects for 3 axes, we have to obtain them now for 4 axes SOLUTION Plane A 1. a 1 = a = a 3 =, c = 1. 1/a 1 = 1/a = 1/a 3 = 0, 1/c = 1 3. No fractions to clear 4. (0001) Plane B 1. a 1 = 1, a = 1, a 3 = 1/, c = 1. 1/a 1 = 1, 1/a = 1, 1/a 3 = , 1/c = 1 3. No fractions to clear 4. (111) 34
35 Determining directions in the hexagonal system is a bit more challenging it is easier to calculate with 3 indices and then simply make up the forth SOLUTION (Continued) Direction C 1. Two points are 0, 0, 1 and 1, 0, 0.. 0, 0, 1,  (1, 0, 0) = 1, 0, 1 3. No fractions to clear or integers to reduce. 4. [101] or [113] Direction D 1. Two points are 0, 1, 0 and 1, 0, 0.. 0, 1, 0,  (1, 0, 0) = 1, 1, 0 3. No fractions to clear or integers to reduce. 4. extension to 4 indices looks easy, but is not! [110]or[1100] How did we get the forth index? All have to be relabeled, say [UVW] are the three indexes, u = 1 / 3 (U V), v = 1 / 3 (VU), t =  1 / 3 (u+v), w = W 35
36 MillerBravais Indices of important directions Typical directions in the hexagonal unit cell, using both threeandfouraxis systems. The dashed lines show that the [110] direction is equivalent to a [010] direction. Densely packed lattice directions in the basal plane (0001), e.g. [100], [010], and [110] have similar MillerBravais indices, important for dislocation slip systems 36
37 37 Now as we have coordinates for lattice points, lattice directions and lattice planes, we can start making crystallographic calculations Good news: everything is easy in the cubic system angle between two different direct [uvw] (or reciprocal (hkl)) space directions So angle between planes is calculated as angle between their normals, if you were to use a protractor (or contact goniometer), you would just measure an angle ß arccos z v u z v u z z v v u u = α arccos l k h l k h l l k k h h = β
38 Bad news: everything gets a bit more difficult in non cubic systems for two reasons, the coordinate axes are no longer perpendicular to each other, the unit vectors of coordinate axes have different length No problem: we have the metric tensor G, a 3 by 3 matrix a abcos γ accos β abcos γ b bccosα accos β bccosα c If cubic simply a a a So angle between lattice directions become α = arccos u' Gv u' Gu v' Gv 38
39 39 Example: what is the angle between [100] and [111] in (tetragonal) ßSn? a = nm, c =0.318nm, Solution: 0) 0 ( ) 0 1 ( a c a a c a a = = nm a Gu u 583 ' = 0. = nm c a a G ) 1 (1 = + + =
40 Putting into relation from above α = arccos u' Gv u' Gu v' Gv α = a arccos = 7. a So that was not all that difficult!!! 40
41 Same basic idea for lattice planes, i.e. their normals which are vectors in reciprocal (or dual) space everything is easy in cubic systems, in other crystal systems we use reciprocal metric tensor, the reciprocal 3 by 3 matrix of the metric tensor b c sin α abc (cosα cos β cos γ ) ab c(cosα cos γ cos β abc a (cosα cos β cos γ a c sin β bc(cos β cos γ cosα ab a c(cosα cos γ bc(cos β cos γ a b sin γ cos β cosα If cubic simply, this also defines the reciproc al lattice 1 a a a α So angle between normals of lattice planes become = arccos h' Gh h' Gk k' Gk 41
42 4 Metric tensor (and its reciprocal) also define reciprocal lattice a b a b c c a c a b c b c b a = = = = = = ) sin ( * ) sin ( * ) sin ( * γ β α It is just a mathematical convenience, particularly useful for interpretation of (Xray and electron diffraction) data d* = H = h a 1 * + ka * + l a 3 *= 1 / d In cubic systems simply: l k h a d hkl + + =
43 Other geometric considerations, valid for all crystal systems, that is the great thing about Miller indices!!! When does a direction lie in a plane? If their dot product is zero, e.g. and (111), = 0 [ 1 01] (1 31) [1 01] But does not lie in as ? 0 What are the indices of the direction that mediated the intersection of two plane? We have to determine cross products ( 1 3) [53] (111) x = 43
44 Centered lattices and structures with more than one lattice point per unit cell (a) Illustration showing sharing of face and corner atoms. (b) The models for simple cubic (SC), body centered cubic (BCC), and facecentered cubic (FCC) unit cells, assuming only one atom per lattice point. 44
45 1 /8 th of an atom R Half of an atom a R R a a Fig. 1.38: The FCC unit cell. The atomic radius is R and the lattice parameter is a 45
46 Determining the Number of Lattice Points in Cubic Crystal Systems Determine the number of lattice points per cell in the cubic crystal systems. If there is only one atom located at each lattice point, calculate the number of atoms per unit cell. SOLUTION In the SC unit cell: lattice point / unit cell = (8 corners)1/8 = 1 In BCC unit cells: lattice point / unit cell = (8 corners)1/8 + (1 center)(1) = In FCC unit cells: lattice point / unit cell = (8 corners)1/8 + (6 faces)(1/) = 4 If there is only on atom per lattice point, as in typical metal structures, the number of atoms per unit cell would be 1,, and 4, for the simple cubic, bodycentered cubic, and facecentered cubic, unit cells, respectively. But there are also many structures with more than one atom per lattice point 46
47 Determining the Relationship between Atomic Radius and Lattice Parameters Determine the relationship between the atomic radius and the lattice parameter in SC, BCC, and FCC structures when one atom is located at each lattice point. The relationships between the atomic radius and the lattice parameter in cubic systems 47
48 SOLUTION Referring to Figure above, we find that atoms touch along the edge of the cube in SC structures. a0 = r In BCC structures, atoms touch along the body diagonal. There are two atomic radii from the center atom and one atomic radius from each of the corner atoms on the body diagonal, so a 0 = 4r In FCC structures, atoms touch along the face diagonal of the cube. There are four atomic radii along this length two radii from the facecentered atom and one radius from each corner, so: a 0 = 3 4r 48
49 THEORETICAL DENSITY, ρ # atoms/unit cell Atomic weight (g/mol) Volume/unit cell (cm 3 /unit cell) ρ = n A V c N A Avogadro's number (6.03 x 10 3 atoms/mol) Example: Copper crystal structure = FCC: 4 atoms/unit cell atomic weight = g/mol (1 amu = 1 g/mol) atomic radius R = 0.18 nm (1 nm = 107 cm) Vc = a 3 ; For FCC, a = 4R/ ; Vc = 4.75 x 103 cm 3 Result: theoretical ρcu = 8.89 g/cm 3 Compare to actual: ρcu = 8.94 g/cm 3 So there must be some real structure in addition! 49
50 Determining the Density of BCC Iron Determine the density of BCC iron, which has a lattice parameter of nm. SOLUTION Atoms/cell =, a 0 = nm = cm Atomic mass = g/mol 3 a 0 Volume of unit cell = = ( cm) 3 = cm 3 /cell Avogadro s number N A = atoms/mol Density ρ = ρ = (3.54 (number of (volume ()(55.847) 10 of = 7.88g / 4 3 )(6.0 atoms/cell)(atomic unit cell)(avog adro' 10 ) mass s of number) cm 3 iron) 50
51 DENSITIES OF MATERIAL CLASSES Metals typically have closepacking (metallic bonding) large atomic mass Ceramics have less dense packing (covalent bonding) often lighter elements Polymers have... poor packing (parts often amorphous) lighter elements (C,H,O) Composites have... intermediate values ρ (g/cm 3 ) Metals/ Alloys Platinum Gold, W Tantalum Silver, Mo Cu,Ni Steels Tin, Zinc Titanium Aluminum Magnesium Graphite/ Ceramics/ Semicond Polymers Composites/ fibers Based on data in Table B1, Callister *GFRE, CFRE, & AFRE are Glass, Carbon, & Aramid FiberReinforced Epoxy composites (values based on 60% volume fraction of aligned fibers in an epoxy matrix). Zirconia Al oxide Diamond Si nitride Glasssoda Concrete Silicon Graphite PTFE Silicone PVC PET PC HDPE, PS PP, LDPE Glass fibers GFRE* Carbon fibers CFRE* Aramid fibers AFRE* Wood 51
52 ATOMIC PACKING FACTOR APF = Volume of atoms in unit cell* Volume of unit cell *assume hard spheres APF for a simple cubic structure = 0.5 a closepacked directions contains 8 x 1/8 = 1 atom/unit cell R=0.5a atoms unit cell APF = 1 volume 4 atom 3 π (0.5a)3 a 3 volume unit cell 5
53 ATOMIC PACKING FACTOR: BCC APF for a bodycentered cubic structure = 0.68 R a atoms unit cell APF = Closepacked directions: length = 4R = 3 a Unit cell contains: x 1/8 = atoms/unit cell 4 3 π ( 3a/4)3 a 3 volume unit cell volume atom 53
54 ATOMIC PACKING FACTOR: FCC APF for a bodycentered cubic structure = 0.74 a atoms unit cell APF = Closepacked directions: length = 4R = a Unit cell contains: 6 x 1/ + 8 x 1/8 = 4 atoms/unit cell π ( a/4)3 a 3 volume unit cell That is the highest possible packing factor!! volume atom 54
55 The hexagonal closepacked (HCP) structure (left) and its unit cell. The packing factor is also 74 %, i.e. the highest possible, just as we had for FCC spheres 55
56 Stacking sequences of closed packed structures, i.e. those with 74 % Packing factor The ABABAB stacking sequence of closepacked planes produces the HCP structure. 56
57 The ABCABCABC stacking sequence of closepacked planes produces the FCC structure. 57
58 Coordination and nearest neighbors Illustration of coordinations in (a) SC six fold and (b) BCC 8 fold unit cells. Six atoms touch each atom in SC, while the eight atoms touch each atom in the BCC unit cell. 58
59 59
60 Lattice Crystal Basis a 90 a Unit cell (a) (b) (c) Unit cell (d) Basis placement in unit cell (0,0) y (1/,1/) x Fig. 1.70: (a) A simple square lattice. The unit cell is a square with a side a. (b) Basis has two atoms. (c) Crystal = Lattice + Basis. The unit cell is a simple square with two atoms. (d) Placement of basis atoms in the crystal unit cell. 60
61 M.C. Escher s two dimensional patterns are filling the whole D space. We can determine a unit cell which happened to be composed off many details, regardless of which periodic detail we use for the choice of the unit cell, these cells will always be identical. So we can think about it in a way that all the details are shrunk into a lattice points and all that remains is the geometrical array of lattice points we had in the previous slide 61
62 6
63 63
64 64
65 65
66 66
67 Interstitial Sites Interstitial sites  Locations between the normal atoms or ions in a crystal into which another  usually different  atom or ion is placed. Typically, the size of this interstitial location is smaller than the atom or ion that is to be introduced. Cubic site  An interstitial position that has a coordination number of eight. An atom or ion in the cubic site touches eight other atoms or ions. Octahedral site  An interstitial position that has a coordination number of six. An atom or ion in the octahedral site touches six other atoms or ions. Tetrahedral site  An interstitial position that has a coordination number of four. An atom or ion in the tetrahedral site touches four other atoms or ions. 67
68 The location of the interstitial sites in cubic unit cells. Only representative sites are shown. 68
69 Interstitial sites are important because we can derive more structures from these basic FCC, BCC, HCP structures by partially or completely different sets of these sites 69
70 Calculating Octahedral Sites How many octahedral sites are there in one FCC unit cell? SOLUTION The octahedral sites include the 1 edges of the unit cell, with the coordinates 1 0, 1 0,0,,0,0,0 1 1,1,0 1 1,,0 1 1,0, 1,0,1 1 1,,1 1 1,1, plus the center position, 1/, 1/, 1/. 1,1,1 1 0,,1 1 0,1, 70
71 SOLUTION (Continued) Each of the sites on the edge of the unit cell is shared between four unit cells, so only 1 / 4 of each site belongs uniquely to each unit cell. Therefore, the number of sites belonging uniquely to each cell is: (1 edges) ( 1 / 4 per cell) + 1 center location = 4 octahedral sites 71
72 How much space is there available to fill the different sites with hard sphere atoms? 7
73 The radios ratios have to be of course the same as the once we discussion in connection with coordination 73
74 Crystal Structures of Ionic Materials Factors that need to be considered in order to understand crystal structures of ionically bonded solids: Ionic Radii for filling of various interstitial sites Electrical Neutrality as a structural principle 74
75 STRUCTURE OF NaCl Compounds: Often have closepacked structures there is more than one atom per lattice point. Structure of NaCl FCC + octahedral Interstitial site filled 75
76 Na + Cl Fig. 1.36: A possible reduced sphere unit cell for the NaCl (rock salt) crystal. An alternative unit cell may have Na+ and Cl interchanged. Examples: AgCl, CaO, CsF, LiF, LiCl, NaF, NaCl, KF, KCl, MgO 76
77 Simple cubic packing with the cube interstitial site filled by another atom, note that there are two atoms per lattice point, i.e. the lattice as such is still simple cubic Cl Cs + Fig. 1.37: A possible reduced sphere unit cell for the CsCl crystal. An alternative unit cell may have Cs + and Cl interchanged. Examples: CsCl, CsBr, CsI, TlCl, TlBr, TlI. 77
78 (a) The zinc blende unit cell, (b) plan view. There is usually a large covalent contribution to these bonds. The coordination is quite low for ionic bonds. 78
79 (a) Fluorite unit cell, (b) plan view. All 8 tetrahedral interstitial sites are filled by F anions, as the formula is CsF, there is three atoms per lattice point. U), ThO and ZrO have the same structure, there is also the antifluorite structure for Li O, Na O, K O with cations and anions reversed 79
80 g Corundum structure of alphaalumina (aai 0 3 ), O in HCP and Al in some of the octahedral interstitial sites, possibly the most widely used ceramic 80
81 Covalent Structures Covalently bonded materials frequently have complex structures in order to satisfy the directional restraints imposed by the bonding. Diamond cubic (DC)  A special type of facecentered cubic crystal structure found in carbon, silicon, αsn, and other covalently bonded materials. 81
82 C a a a Fig. 1.33: The diamond unit cell is cubic. The cell has eight atoms. Grey Sn (αsn) and the elemental semiconductors Ge and Si have this crystal structure. 8
83 S a Zn a a Fig. 1.34: The Zinc blende (ZnS) cubic crystal structure. Many important compound crystals have the zinc blende structure. Examples: AlAs, GaAs, GaP, GaSb, InAs, InP, InSb, ZnS, ZnTe. 83
84 The siliconoxygen tetrahedron and the resultant ß cristobalite form of silica. Note: there is six atom at every lattice point, i.e. one Si in the center, 4 O within the tetrahedron and 4 times ¼ Si at the apexes of each tetrahedron 84
85 The unit cell of crystalline polyethylene, Orthorhombic, there are typically many defects in polymer crystals 85
86 METALLIC CRYSTALS tend to be densely packed. have several reasons for dense packing: Typically, only one element is present, so all atomic radii are the same. Metallic bonding is not directional. Nearest neighbor distances tend to be small in order to lower bond energy. have the simplest crystal structures. We will revisit the two closest packed structures and give some examples for each of them 86
87 (a) FCC Unit Cell R a a a (b) a (c) Fig. 1.30: (a) The crystal structure of copper is Face Centered Cubic (FCC). The atoms are positioned at well defined sites arranged periodically and there is a long range order in the crystal. (b) An FCC unit cell with closed packed spheres. (c) Reduced sphere representation of the FCC unit cell. Examples: Ag, Al, Au, Ca, Cu, γfe (>91 C), Ni, Pd, Pt, Rh 87
88 Layer B (a) a (c) Layer A Layer B Layer A c Layer A (d) (b) Examples: Be, Mg, αti ( < 88 C ), Cr, Co, Zn, Zr, Cd Layer A Be very careful, the yellow and blue spheres represent one and the same type of atoms Fig. 1.3: The Hexagonal Close Packed (HCP) Crystal Structure. (a) The Hexagonal Close Packed (HCP) Structure. A collection of many Zn atoms. Color difference distinguishes layers (stacks). (b) The stacking sequence of closely packed layers is ABAB (c) A unit cell with reduced spheres (d) The smallest unit cell with reduced spheres. 88
89 What is steel? It s not an element, it s an intestinal alloy, about 1 C atom every 50 Fe atoms, i.e. 0.4 weight % C So the crystal structure is BCC, as it is Fe at room temperature, every now and then a much smaller c atom fits into one of the cubic interstitial sites and this increases the strength from about 15 MPa to more than 1500 MPa How is that little amount of C accomplishing so much? More about things such as this in next lecture on lattice defects 89
90 SUMMARY Crystals Atoms typically assemble into crystals some materials e.g. glass are amorphous, i.e. have only short range order We can predict the density of a material, provided we know the atomic weight, atomic radius, and crystal geometry (e.g., FCC, BCC, HCP). Material properties generally vary with single crystal orientation (i.e., they are anisotropic), but properties are frequently quite nondirectional (i.e., they are isotropic) in polycrystals with randomly oriented grains as e.g. in steel and other engineering materials 90
91 Diffraction Techniques for Crystal Structure Analysis Diffraction  The constructive interference, or reinforcement, of a beam of xrays or electrons interacting with a material. The diffracted beam provides useful information concerning the structure of the material. Bragg s law  The relationship describing the angle? at which a beam of xrays of a particular wavelength diffracts from crystallographic planes of a given interplanar spacing. In a diffractometer a moving xray detector records the? angles at which the beam is diffracted, giving a characteristic diffraction pattern 91
92 Lattice constants range from about 0.1 nm to some nm. Most crystals lattice constants are in the 15 nm range, since crystals are periodic, they are the ideal diffraction grating for Xrays, Max von Laue s 1914 Nobel prize that proved both, crystals are periodic 3D arrangements of atoms and Xrays are waves (well waveparticles actually) 9
93 The diffraction angle is always? Bragg s law: n l = d hkl sin? n the order of reflection can be dropped by allowing indices for hkl that are not smallest integers, i.e. HKL 93
94 Single crystal diffractometers are more sophisticated 94
95 Powder diffractometers (for polycrystalline powder) are less sophisticated and can be found in many places 95
96 (a) sketch of a diffractometer viewed from above, showing powder sample, incident and diffracted beams. (b) diffraction pattern obtained from a sample of gold powder, notice the Miller indices of the diffracting crystal planes 96
97 1 detector incoming Xrays extra distance travelled by wave θ 1 θ outgoing Xrays λ d reflections must be in phase to detect signal spacing between planes Measurement of: reflection angles (Bragg angles), θ, for Xrays provide atomic spacing, d. xray intensity (from detector) θc d=nλ/sinθc θ 97
98 (a) Destructive and (b) reinforcing (constructive) interference between xrays reflected on a set of planes. Reinforcement occurs only at angles that satisfy Bragg s law. l = d HKL sin? No other Xray diffraction peaks occur 98
99 Xray Diffraction for an forensic examination The results of a xray diffraction experiment on some metal powder found at a crime scene using characteristic xrays with? = Å (a radiation obtained from molybdenum (Mo) target) show that diffracted peaks occur at the following? angles: Determine the indices of the plane producing each peak, and from that the lattice parameter of the material and from that identify the material (you know it is some metal so it is a good guess to assume the crystals in the powder are cubic) 99
100 SOLUTION λ = d HKL sin? d HKL = H 1 + K + L λ ( ) = d HKL sin θ = ( Ha * + Kb* + Lc*) = ( d ) 1 * 1 HKL = r g We first determine the sin? value for each peak, then divide through by the lowest denominator, , guess the indices 100
101 SOLUTION (Continued) We could then use? values for any of the peaks to calculate the interplanar spacing and thus the lattice parameter. Picking peak 8:? = 59.4 or? = 9.71 d 400 = λ sin θ = sin(9.71) = Å a 0 = d 400 h + k + l = ( )(4) =.868 Å This is the lattice parameter for bodycentered cubic iron. So the gardener did steal the cookies only kidding Since out of all metals only Po has the simple cubic structure, and we do know our material was not radioactive and difficult to obtain, we didn t check for an indexing scheme for a single cubic lattice, it would have gotten us nowhere anyway 101
102 There are certain systematic absences of reflections You may have noticed that there are no (hkl) triplets with h+k+l = odd. Laue s kinematical theory of Xray diffraction (191) explains why, different structures have forbidden reflections, i.e. reflections that do not show up in diffraction but these planes do of course exist in the crystals, it is just that diffraction on them is destructive Simple cubic crystals have no forbidden reflections 10
103 A TEM micrograph of an aluminum alloy (Al7055) sample. The diffraction pattern at the right shows large bright spots that represent diffraction from the main aluminum matrix grains. The smaller spots originate from the nanoscale crystals of another compound that is present in the aluminum alloy. 103
104 (In,Ga)P, an important semiconductor for visible light lasers can show a variety of atomic ordering The very same thing, i.e. atomic ordering exist in metals as well 104
105 IIVI semiconductors with atomic ordering, (Cd,Zn)Se quantum dots in ZnSe, [001] plan view (Cd,Mn,Zn)Se quantum dots in <110> cross section 105
106 Unknown crystallographic phase in (In,Ga)(Sb,As) quantum dots in InAs matrix, a Fourier transform power spectrum of a high resolution TEM images replaces frequently a diffraction pattern as much of the information is contained in such calculated images 106
107 False color convergent beam electron diffraction pattern, From the symmetry of the lines (Kikuchi lines), the crystal system can be determined From the fine structure of the diffraction disk, the space group can be determined Works for extremely tiny specs of matter, perhaps nm across 107
108 Wow, what is that? It can t be a crystal as it obviously has a five fold symmetry, it is not amorphous either as it clearly has a diffraction pattern? It s a quasicrystal, i.e. and entity with short range order (as amorphous and crystalline materials) and long range order (as a crystal), the crucial difference is, the long range order is non periodic 108
109 Crystallographic work can also be done in modern SEMs! Electron backscatter (Kikuchi) diffraction (EBSD), here of a Si crystal 109
110 scanning probe microscopy, STM, AFM, Atoms can be arranged and imaged! Carbon monoxide molecules arranged on a platinum (111) surface. Iron atoms arranged on a copper (111) surface. These Kanji characters represent the word atom. Something more useful, the square of the quantum mechanical wave function of an electron that is trapped in a cage of Cu atoms 110
Chapter Outline. How do atoms arrange themselves to form solids?
Chapter Outline How do atoms arrange themselves to form solids? Fundamental concepts and language Unit cells Crystal structures Simple cubic Facecentered cubic Bodycentered cubic Hexagonal closepacked
More informationChapter 3: The Structure of Crystalline Solids
Sapphire: cryst. Al 2 O 3 Insulin : The Structure of Crystalline Solids Crystal: a solid composed of atoms, ions, or molecules arranged in a pattern that is repeated in three dimensions A material in which
More informationCrystal Symmetries METE 327 Physical Metallurgy Copyright 2008 Loren A. Jacobson 5/16/08
Crystal Symmetries Why should we be interested? Important physical properties depend on crystal structure Conductivity Magnetic properties Stiffness Strength These properties also often depend on crystal
More informationCHAPTER 3 THE STRUCTURE OF CRYSTALLINE SOLIDS PROBLEM SOLUTIONS
CHAPTER THE STRUCTURE OF CRYSTALLINE SOLIDS PROBLEM SOLUTIONS Fundamental Concepts.6 Show that the atomic packing factor for HCP is 0.74. The APF is just the total sphere volumeunit cell volume ratio.
More informationChapter 3: Structure of Metals and Ceramics. Chapter 3: Structure of Metals and Ceramics. Learning Objective
Chapter 3: Structure of Metals and Ceramics Chapter 3: Structure of Metals and Ceramics Goals Define basic terms and give examples of each: Lattice Basis Atoms (Decorations or Motifs) Crystal Structure
More informationRelevant Reading for this Lecture... Pages 8387.
LECTURE #06 Chapter 3: Xray Diffraction and Crystal Structure Determination Learning Objectives To describe crystals in terms of the stacking of planes. How to use a dot product to solve for the angles
More informationSolid State Theory Physics 545
Solid State Theory Physics 545 CRYSTAL STRUCTURES Describing periodic structures Terminology Basic Structures Symmetry Operations Ionic crystals often have a definite habit which gives rise to particular
More informationChapter 3. 1. 3 types of materials amorphous, crystalline, and polycrystalline. 5. Same as #3 for the ceramic and diamond crystal structures.
Chapter Highlights: Notes: 1. types of materials amorphous, crystalline, and polycrystalline.. Understand the meaning of crystallinity, which refers to a regular lattice based on a repeating unit cell..
More informationCrystals are solids in which the atoms are regularly arranged with respect to one another.
Crystalline structures. Basic concepts Crystals are solids in which the atoms are regularly arranged with respect to one another. This regularity of arrangement can be described in terms of symmetry elements.
More informationThe Crystal Structures of Solids
The Crystal Structures of Solids Crystals of pure substances can be analyzed using Xray diffraction methods to provide valuable information. The type and strength of intramolecular forces, density, molar
More informationMaterials Science and Engineering Department MSE , Sample Test #1, Spring 2010
Materials Science and Engineering Department MSE 200001, Sample Test #1, Spring 2010 ID number First letter of your last name: Name: No notes, books, or information stored in calculator memories may be
More informationChapters 2 and 6 in Waseda. Lesson 8 Lattice Planes and Directions. Suggested Reading
Analytical Methods for Materials Chapters 2 and 6 in Waseda Lesson 8 Lattice Planes and Directions Suggested Reading 192 Directions and Miller Indices Draw vector and define the tail as the origin. z Determine
More informationA crystalline solid is one which has a crystal structure in which atoms or ions are arranged in a pattern that repeats itself in three dimensions.
CHAPTER ATOMIC STRUCTURE AND BONDING. Define a crstalline solid. A crstalline solid is one which has a crstal structure in which atoms or ions are arranged in a pattern that repeats itself in three dimensions..2
More informationReading. Chapter 12 in DeGraef and McHenry Chapter 3i in Engler and Randle
Class 17 Xray Diffraction Chapter 1 in DeGraef and McHenry Chapter 3i in Engler and Randle Reading Chapter 6 in DeGraef and McHenry (I WILL ASSUME THAT YOU KNOW ABOUT THIS CONCEPT ALREADY! IF NOT, READ
More informationExperiment: Crystal Structure Analysis in Engineering Materials
Experiment: Crystal Structure Analysis in Engineering Materials Objective The purpose of this experiment is to introduce students to the use of Xray diffraction techniques for investigating various types
More informationChem 106 Thursday Feb. 3, 2011
Chem 106 Thursday Feb. 3, 2011 Chapter 13: The Chemistry of Solids Phase Diagrams  (no BornHaber cycle) 2/3/2011 1 Approx surface area (Å 2 ) 253 258 Which C 5 H 12 alkane do you think has the highest
More informationLecture 2. Surface Structure
Lecture 2 Surface Structure Quantitative Description of Surface Structure clean metal surfaces adsorbated covered and reconstructed surfaces electronic and geometrical structure References: 1) Zangwill,
More informationCHAPTER 4 IMPERFECTIONS IN SOLIDS PROBLEM SOLUTIONS
41 CHAPTER 4 IMPERFECTIONS IN SOLIDS PROBLEM SOLUTIONS Vacancies and SelfInterstitials 4.1 In order to compute the fraction of atom sites that are vacant in copper at 1357 K, we must employ Equation
More informationXRay Diffraction HOW IT WORKS WHAT IT CAN AND WHAT IT CANNOT TELL US. Hanno zur Loye
XRay Diffraction HOW IT WORKS WHAT IT CAN AND WHAT IT CANNOT TELL US Hanno zur Loye Xrays are electromagnetic radiation of wavelength about 1 Å (1010 m), which is about the same size as an atom. The
More informationChapter 2 Crystal Lattices and Reciprocal Lattices
Chapter 2 Crystal Lattices and Reciprocal Lattices Abstract In this chapter, the basic unit vectors in real space and the basic unit vectors in reciprocal space, as well as their reciprocal relationships,
More informationCHAPTER 3: CRYSTAL STRUCTURES
CHAPTER 3: CRYSTAL STRUCTURES Crystal Structure: Basic Definitions  lecture Calculation of material density selfprep. Crystal Systems lecture + selfprep. Introduction to Crystallography lecture + selfprep.
More informationCrystal Structure Determination I
Crystal Structure Determination I Dr. Falak Sher Pakistan Institute of Engineering and Applied Sciences National Workshop on Crystal Structure Determination using Powder XRD, organized by the Khwarzimic
More informationThe University of Western Ontario Department of Physics and Astronomy P2800 Fall 2008
P2800 Fall 2008 Questions (Total  20 points): 1. Of the noble gases Ne, Ar, Kr and Xe, which should be the most chemically reactive and why? (0.5 point) Xenon should be most reactive since its outermost
More informationCHEM 10113, Quiz 7 December 7, 2011
CHEM 10113, Quiz 7 December 7, 2011 Name (please print) All equations must be balanced and show phases for full credit. Significant figures count, show charges as appropriate, and please box your answers!
More informationXray diffraction: theory and applications to materials science and engineering. Luca Lutterotti
Xray diffraction: theory and applications to materials science and engineering Luca Lutterotti luca.lutterotti@unitn.it Program Part 1, theory and methodologies: General principles of crystallography
More informationMAE 20 Winter 2011 Assignment 2 solutions
MAE 0 Winter 0 Assignment solutions. List the point coordinates of the titanium, barium, and oxygen ions for a unit cell of the perovskite crystal structure (Figure.6). In Figure.6, the barium ions are
More informationIntroduction to Materials Science, Chapter 13, Structure and Properties of Ceramics. Chapter Outline: Ceramics
Chapter Outline: Ceramics Chapter 13: Structure and Properties of Ceramics Crystal Structures Silicate Ceramics Carbon Imperfections in Ceramics Optional reading: 13.6 13.10 Chapter 14: Applications and
More informationPOWDER XRAY DIFFRACTION: STRUCTURAL DETERMINATION OF ALKALI HALIDE SALTS
EXPERIMENT 4 POWDER XRAY DIFFRACTION: STRUCTURAL DETERMINATION OF ALKALI HALIDE SALTS I. Introduction The determination of the chemical structure of molecules is indispensable to chemists in their effort
More informationThis is Solids, chapter 12 from the book Principles of General Chemistry (index.html) (v. 1.0).
This is Solids, chapter 12 from the book Principles of General Chemistry (index.html) (v. 1.0). This book is licensed under a Creative Commons byncsa 3.0 (http://creativecommons.org/licenses/byncsa/
More information12.524 2003 Lec 17: Dislocation Geometry and Fabric Production 1. Crystal Geometry
12.524 2003 Lec 17: Dislocation Geometry and Fabric Production 1. Bibliography: Crystal Geometry Assigned Reading: [Poirier, 1985]Chapter 2, 4. General References: [Kelly and Groves, 1970] Chapter 1. [Hirth
More informationThe Structure of solids.
Chapter S. The Structure of solids. After having studied this chapter, the student will be able to: 1. Distinguish between a crystal structure and an amorphous structure. 2. Describe the concept of a unit
More information2Introduction to Structure and Bonding in Materials
2Introduction to Structure and Bonding in Materials 21SubAtomic Structure Electrons and their interaction with the nucleus of the atom. The Bohr model is a simplified view of the arrangement of subatomic
More informationType of Solid Particles Attractive Force Properties Examples. ionic positive ions electrostatic solid poor conductor NaCl KNO 3
Soids&Materials 1 Solids & Materials Summary of Properties and Types of Solids Type of Solid Particles Attractive Force Properties Examples ionic positive ions electrostatic solid poor conductor NaCl KNO
More informationImperfections in atomic arrangements
MME131: Lecture 8 Imperfections in atomic arrangements Part 1: 0D Defects A. K. M. B. Rashid Professor, Department of MME BUET, Dhaka Today s Topics Occurrence and importance of crystal defects Classification
More informationSample Exercise 12.1 Calculating Packing Efficiency
Sample Exercise 12.1 Calculating Packing Efficiency It is not possible to pack spheres together without leaving some void spaces between the spheres. Packing efficiency is the fraction of space in a crystal
More informationBasic Concepts of Crystallography
Basic Concepts of Crystallography Language of Crystallography: Real Space Combination of local (point) symmetry elements, which include angular rotation, centersymmetric inversion, and reflection in mirror
More informationWafer Manufacturing. Reading Assignments: Plummer, Chap 3.1~3.4
Wafer Manufacturing Reading Assignments: Plummer, Chap 3.1~3.4 1 Periodic Table Roman letters give valence of the Elements 2 Why Silicon? First transistor, Shockley, Bardeen, Brattain1947 Made by Germanium
More informationEach grain is a single crystal with a specific orientation. Imperfections
Crystal Structure / Imperfections Almost all materials crystallize when they solidify; i.e., the atoms are arranged in an ordered, repeating, 3dimensional pattern. These structures are called crystals
More informationSolid State Device Fundamentals
Solid State Device Fundamentals ENS 345 Lecture Course by Alexander M. Zaitsev alexander.zaitsev@csi.cuny.edu Tel: 718 982 2812 Office 4N101b 1 Solids Three types of solids, classified according to atomic
More informationRetained Austenite: NonDestructive Analysis by XRD and ASTM E Dr. Alessandro Torboli  XRay Marketing Manager
Retained Austenite: NonDestructive Analysis by XRD and ASTM E97503 Dr. Alessandro Torboli  XRay Marketing Manager Outline Introduction to XRay Diffraction Retained Austenite Retained Austenite by
More informationIt is unaffected by electric and magnetic fields (as is all electromagnetic radiation e.g. light).
γradiation Electromagnetic radiation with very short wavelength, smaller than even Xrays  arises from most nuclear disintegrations. It causes no change in atomic structure upon emission. It is unaffected
More informationClasses of materials
Classes of materials POLYMERS CERAMICS METALS DUCTILITY Varies Poor Good CONDUCTIVITY (ELECTRICAL & THERMAL) Low Low High HARDNESS/STRENGTH Low medium Very high Medium high CORROSION RESISTANCE Fair good
More informationLiquids and Solids. AP Chemistry Chapter 10. 9/20/2009 Jodi Grack; Wayzata High School; images used with permission from Zumdahl
Liquids and Solids AP Chemistry Chapter 10 Liquids and Solids Gases are much easier to study because molecules move independent of each other. In liquids and solids forces between molecules become very
More information3. What would you predict for the intensity and binding energy for the 3p orbital for that of sulfur?
PSI AP Chemistry Periodic Trends MC Review Name Periodic Law and the Quantum Model Use the PES spectrum of Phosphorus below to answer questions 13. 1. Which peak corresponds to the 1s orbital? (A) 1.06
More informationUNIT 1 THE SOLID STATE VERY SHORT ANSWER TYPE QUESTIONS (1 MARKS)
UNIT 1 THE SOLID STATE VERY SHORT ANSWER TYPE QUESTIONS (1 MARKS) Q1. How many spheres are in contact with each other in a single plane of a close packed structure? A1. Six(6). Q2.Name the two closest
More informationChapter 13 The Chemistry of Solids
Chapter 13 The Chemistry of Solids Jeffrey Mack California State University, Sacramento Metallic & Ionic Solids Crystal Lattices Regular 3D arrangements of equivalent LATTICE POINTS in space. Lattice
More informationTheory of XRay Diffraction. Kingshuk Majumdar
Theory of XRay Diffraction Kingshuk Majumdar Contents Introduction to XRays Crystal Structures: Introduction to Lattices Different types of lattices Reciprocal Lattice Index Planes XRay Diffraction:
More informationElementary Crystallography for XRay Diffraction
Introduction Crystallography originated as the science of the study of crystal forms. With the advent of the xray diffraction, the science has become primarily concerned with the study of atomic arrangements
More informationME 612 Metal Forming and Theory of Plasticity. 1. Introduction
Metal Forming and Theory of Plasticity Yrd.Doç. e mail: azsenalp@gyte.edu.tr Makine Mühendisliği Bölümü Gebze Yüksek Teknoloji Enstitüsü In general, it is possible to evaluate metal forming operations
More informationXray Diffraction and EBSD
Xray Diffraction and EBSD Jonathan Cowen Swagelok Center for the Surface Analysis of Materials Case School of Engineering Case Western Reserve University October 27, 2014 Outline Xray Diffraction (XRD)
More informationThe atomic packing factor is defined as the ratio of sphere volume to the total unit cell volume, or APF = V S V C. = 2(sphere volume) = 2 = V C = 4R
3.5 Show that the atomic packing factor for BCC is 0.68. The atomic packing factor is defined as the ratio of sphere volume to the total unit cell volume, or APF = V S V C Since there are two spheres associated
More informationPeriodic Table. inert gases. Columns: Similar Valence Structure. give up 1e  give up 2e  Oaccept 2e accept 1e  give up 3e 
Periodic Table give up 1e  give up 2e  give up 3e  H Li Be Na Mg K Ca Columns: Similar Valence Structure Sc Oaccept 2e accept 1e  inert gases S Se F Cl Br He Ne Ar Kr Adapted from Fig. 2.6, Callister
More informationWe shall first regard the dense sphere packing model. 1.1. Draw a two dimensional pattern of dense packing spheres. Identify the twodimensional
Set 3: Task 1 and 2 considers many of the examples that are given in the compendium. Crystal structures derived from sphere packing models may be used to describe metals (see task 2), ionical compounds
More informationUnit 12 Practice Test
Name: Class: Date: ID: A Unit 12 Practice Test Multiple Choice Identify the choice that best completes the statement or answers the question. 1) A solid has a very high melting point, great hardness, and
More information305 ATOMS, ELEMENTS, AND MINERALS
DATE DUE: Name: Instructor: Ms. Terry J. Boroughs Geology 305 ATOMS, ELEMENTS, AND MINERALS Instructions: Read each question carefully before selecting the BEST answer. Use GEOLOGIC VOCABULARY where APPLICABLE!
More informationMatter, Materials, Crystal Structure and Bonding. Chris J. Pickard
Matter, Materials, Crystal Structure and Bonding Chris J. Pickard Why should a theorist care? Where the atoms are determines what they do Where the atoms can be determines what we can do Overview of Structure
More informationSolid Type of solid Type of particle
QUESTION (2015:3) Complete the table below by stating the type of solid, the type of particle, and the attractive forces between the particles in each solid. Solid Type of solid Type of particle Cu(s)
More informationChapter 10  Liquids and Solids
Chapter 10  Liquids and Solids 10.1 Intermolecular Forces A. DipoleDipole Forces 1. Attraction between molecules with dipole moments a. Maximizes (+)  (  ) interactions b. Minimizes (+)  (
More informationThe Periodic Table, Electron Configuration & Chemical Bonding. Lecture 7
The Periodic Table, Electron Configuration & Chemical Bonding Lecture 7 Electrons We will start to look at the periodic table by focusing on the information it gives about each element s electrons. How
More informationStructure of Metals 110
Structure of Metals 110 Welcome to the Tooling University. This course is designed to be used in conjunction with the online version of this class. The online version can be found at http://www.toolingu.com.
More informationCRYSTALLINE SOLIDS IN 3D
CRYSTALLINE SOLIDS IN 3D Andrew Baczewski PHY 491, October 7th, 2011 OVERVIEW First  are there any questions from the previous lecture? Today, we will answer the following questions: Why should we care
More informationLMB Crystallography Course, 2013. Crystals, Symmetry and Space Groups Andrew Leslie
LMB Crystallography Course, 2013 Crystals, Symmetry and Space Groups Andrew Leslie Many of the slides were kindly provided by Erhard Hohenester (Imperial College), several other illustrations are from
More informationLösungen Übung Verformung
Lösungen Übung Verformung 1. (a) What is the meaning of T G? (b) To which materials does it apply? (c) What effect does it have on the toughness and on the stress strain diagram? 2. Name the four main
More informationDefects Introduction. Bonding + Structure + Defects. Properties
Defects Introduction Bonding + Structure + Defects Properties The processing determines the defects Composition Bonding type Structure of Crystalline Processing factors Defects Microstructure Types of
More informationXray Diffraction (XRD)
Xray Diffraction (XRD) 1.0 What is Xray Diffraction 2.0 Basics of Crystallography 3.0 Production of Xrays 4.0 Applications of XRD 5.0 Instrumental Sources of Error 6.0 Conclusions Bragg s Law n l =2dsinq
More informationMicroscopy and Nanoindentation. Combining Orientation Imaging. to investigate localized. deformation behaviour. Felix Reinauer
Combining Orientation Imaging Microscopy and Nanoindentation to investigate localized deformation behaviour Felix Reinauer René de Kloe Matt Nowell Introduction Anisotropy in crystalline materials Presentation
More informationLecture 2: Semiconductors: Introduction
Lecture 2: Semiconductors: Introduction Contents 1 Introduction 1 2 Band formation in semiconductors 2 3 Classification of semiconductors 5 4 Electron effective mass 10 1 Introduction Metals have electrical
More informationIonic and Metallic Bonding
Ionic and Metallic Bonding BNDING AND INTERACTINS 71 Ions For students using the Foundation edition, assign problems 1, 3 5, 7 12, 14, 15, 18 20 Essential Understanding Ions form when atoms gain or lose
More information100% ionic compounds do not exist but predominantly ionic compounds are formed when metals combine with nonmetals.
2.21 Ionic Bonding 100% ionic compounds do not exist but predominantly ionic compounds are formed when metals combine with nonmetals. Forming ions Metal atoms lose electrons to form +ve ions. Nonmetal
More informationb) What is the trend in melting point as one moves up the group in alkali metals? Explain.
Problem Set 2 Wed May 25, 2011 1. What is the rough trend in the number of oxidation states available to the elements (excluding the noble gases) as you move a) to the right and b) down the periodic table?
More informationUse the PES spectrum of Phosphorus below to answer questions 13.
Use the PES spectrum of Phosphorus below to answer questions 13. 1. Which peak corresponds to the 1s orbital? (A) 1.06 (B) 1.95 (C) 13.5 (D) 18.7 (E) 208 2. Which peak corresponds to the valence 3p orbital?
More informationNext, solid silicon is separated from other solid impurities by treatment with hydrogen chloride at 350 C to form gaseous trichlorosilane (SiCl 3 H):
University Chemistry Quiz 5 2014/12/25 1. (5%) What is the coordination number of each sphere in (a) a simple cubic cell, (b) a bodycentered cubic cell, and (c) a facecentered cubic cell? Assume the
More informationFundamentals of grain boundaries and grain boundary migration
1. Fundamentals of grain boundaries and grain boundary migration 1.1. Introduction The properties of crystalline metallic materials are determined by their deviation from a perfect crystal lattice, which
More information305 ATOMS, ELEMENTS, AND MINERALS
DATE DUE: Name: Instructor: Ms. Terry J. Boroughs Geology 305 ATOMS, ELEMENTS, AND MINERALS Instructions: Read each question carefully before selecting the BEST answer. Use GEOLOGIC VOCABULARY where APPLICABLE!
More informationCrystal Structure of High Temperature Superconductors. Marie Nelson East Orange Campus High School NJIT Professor: Trevor Tyson
Crystal Structure of High Temperature Superconductors Marie Nelson East Orange Campus High School NJIT Professor: Trevor Tyson Introduction History of Superconductors Superconductors are material which
More informationChapter Outline. Review of Atomic Structure Electrons, Protons, Neutrons, Quantum mechanics of atoms, Electron states, The Periodic Table
Review of Atomic Structure Electrons, Protons, Neutrons, Quantum mechanics of atoms, Electron states, The Periodic Table Atomic Bonding in Solids Bonding Energies and Forces Periodic Table Chapter Outline
More information in a typical metal each atom contributes one electron to the delocalized electron gas describing the conduction electrons
Free Electrons in a Metal  in a typical metal each atom contributes one electron to the delocalized electron gas describing the conduction electrons  if these electrons would behave like an ideal gas
More informationBasics in Xray Diffraction and Special Application
Basics in Xray Diffraction and Special Application Introduction: Xray Diffraction (XRD) helps one to reach the science at atomic scale in the analysis of crystal structure, chemical composition, and
More information1 Electrons and Chemical Bonding
CHAPTER 1 1 Electrons and Chemical Bonding SECTION Chemical Bonding BEFORE YOU READ After you read this section, you should be able to answer these questions: What is chemical bonding? What are valence
More informationExplain the ionic bonds, covalent bonds and metallic bonds and give one example for each type of bonds.
Problem 1 Explain the ionic bonds, covalent bonds and metallic bonds and give one example for each type of bonds. Ionic Bonds Two neutral atoms close to each can undergo an ionization process in order
More informationXray thinfilm measurement techniques
Technical articles Xray thinfilm measurement techniques II. Outofplane diffraction measurements Toru Mitsunaga* 1. Introduction A thinfilm sample is twodimensionally formed on the surface of a substrate,
More informationGeo 101 (Minerals  Unit 2)
 A mineral is: 1. Natural. 2. Inorganic solid. 3. Has a chemical composition. 4. Has a crystalline structure. Geo 101 (Minerals  Unit 2)  The two important properties of a mineral are: 1. Chemical composition.
More informationName: Class: Date: Multiple Choice Identify the letter of the choice that best completes the statement or answers the question.
Class: Date: Minerals Study Guide Modified True/False Indicate whether the sentence or statement is true or false. If false, change the identified word or phrase to make the sentence or statement true.
More informationEarth Sciences: Course Presenters
Earth Sciences: Course Presenters 625102 Geology Dr Stephen Gallagher Prof Andrew Gleadow Dr Malcolm Wallace Prof Ian Plimer Course Coordinator Room 214 Series  Lecture Topics 1. Mineralogy and Crystals
More informationThe Nature of Chemistry
CHAPTER 1 The Nature of Chemistry Objectives You will be able to do the following. 1. Describe how science in general is done. 2. Given a description of a property of a substance, identify the property
More informationCoordination and Pauling's Rules
Page 1 of 8 EENS 2110 Tulane University Mineralogy Prof. Stephen A. Nelson Coordination and Pauling's Rules This document last updated on 24Sep2013 The arrangement of atoms in a crystal structure not
More informationNPTEL: STRUCTURE OF MATERIALS Instructor: Anandh Subramaniam [Lecture1 to Lecture45] 1. Overview (C1) (Time: 49:06)
NPTEL: STRUCTURE OF MATERIALS Instructor: Anandh Subramaniam [Lecture1 to Lecture45] Lec Chapter 1. Overview (C1) (Time: 49:06) 2. Geometry of Crystals: Symmetry, Lattices (C2) (Time: 1:08:58) 3. (Time:
More informationEXPERIMENT 4. Microwave Experiments. Introduction. Experimental Procedure. Part 1 : Double Slit
EXPERIMENT 4 Microwave Experiments Introduction Microwaves are electromagnetic radiation in the centimeter range of wavelengths. As such, they, like light, will exhibit typical wave properties like interference
More informationCrystallographic Points, Directions, and Planes. ISSUES TO ADDRESS... a v. Points, Directions, and Planes in Terms of Unit Cell Vectors
Crstallographic Points, Directions, and Planes. Points, Directions, and Planes in Terms of Unit Cell Vectors ISSUES TO ADDRESS... How to define points, directions, planes, as well as linear, planar, and
More informationLecture 01: Crystalline and Noncrystalline solids
Lecture 01: Crystalline and Noncrystalline solids Introduction Matter can be subdivided into two statessolid and fluid, of which the later is subdivided into liquid and gaseous state. Matter can also
More information11 Chemical Bonds: The Formation of Compounds from Atoms. Chapter Outline. Periodic Trends in Atomic Properties. Periodic Trends in Atomic Properties
11 Chemical Bonds The Formation of Compounds from Atoms Chapter Outline 11.1 11.2 Lewis Structures of Atoms 11.3 The Ionic Bond Transfer of Electrons from One Atom to Another 11.4 Predicting Formulas of
More informationCHAPTER 10: INTERMOLECULAR FORCES: THE UNIQUENESS OF WATER Problems: 10.2, 10.6,10.1510.33, 10.3510.40, 10.5610.60, 10.10110.
CHAPTER 10: INTERMOLECULAR FORCES: THE UNIQUENESS OF WATER Problems: 10.2, 10.6,10.1510.33, 10.3510.40, 10.5610.60, 10.10110.102 10.1 INTERACTIONS BETWEEN IONS Ionion Interactions and Lattice Energy
More informationB) atomic number C) both the solid and the liquid phase D) Au C) Sn, Si, C A) metal C) O, S, Se C) In D) tin D) methane D) bismuth B) Group 2 metal
1. The elements on the Periodic Table are arranged in order of increasing A) atomic mass B) atomic number C) molar mass D) oxidation number 2. Which list of elements consists of a metal, a metalloid, and
More informationTopic 4. Chemical bonding and structure
Topic 4. Chemical bonding and structure There are three types of strong bonds: Ionic Covalent Metallic Some substances contain both covalent and ionic bonding or an intermediate. 4.1 Ionic bonding Ionic
More informationName period AP chemistry Unit 2 worksheet Practice problems
Name period AP chemistry Unit 2 worksheet Practice problems 1. What are the SI units for a. Wavelength of light b. frequency of light c. speed of light Meter hertz (s 1 ) m s 1 (m/s) 2. T/F (correct
More informationAtoms and Elements. Atoms: Learning Goals. Chapter 3. Atoms and Elements; Isotopes and Ions; Minerals and Rocks. Clicker 1. Chemistry Background?
Chapter 3 Atoms Atoms and Elements; Isotopes and Ions; Minerals and Rocks A Review of Chemistry: What geochemistry tells us Clicker 1 Chemistry Background? A. No HS or College Chemistry B. High School
More informationMinerals in granite. The igneous rock granite is composed of many separate grains of several main minerals. Figure 2.1
Minerals in granite The igneous rock granite is composed of many separate grains of several main minerals Figure 2.1 What is a mineral? Naturally occurring solid Specific chemical composition Crystal structure
More informationFormation of solids from solutions and melts
Formation of solids from solutions and melts Solids from a liquid phase. 1. The liquid has the same composition as the solid. Formed from the melt without any chemical transformation. Crystallization and
More informationElectroceramics Prof. Ashish Garg Department of Material Science and Engineering Indian Institute of Technology, Kanpur.
Electroceramics Prof. Ashish Garg Department of Material Science and Engineering Indian Institute of Technology, Kanpur Lecture  3 Okay, so in this third lecture we will just review the last lecture,
More information14:635:407:02 Homework III Solutions
14:635:407:0 Homework III Solutions 4.1 Calculate the fraction of atom sites that are vacant for lead at its melting temperature of 37 C (600 K). Assume an energy for vacancy formation of 0.55 ev/atom.
More information